Corrosion Behavior of High-Mn Austenitic Fe–Mn–Al–Cr–C Steels in NaCl and NaOH Solutions

The corrosion behavior of austenitic Fe–Mn–Al–Cr–C twinning-induced plasticity (TWIP) and microband-induced plasticity (MBIP) steels with different alloying elements ranging from 22.6–30 wt.% Mn, 5.2–8.5 wt.% Al, 3.1–5.1 wt.% Cr, to 0.68–1.0 wt.% C was studied in 3.5 wt.% NaCl (pH 7) and 10 wt.% NaOH (pH 14) solutions. The results obtained using potentiodynamic polarization and electrochemical impedance spectroscopy (EIS) techniques, alongside optical microscopy analysis, revealed pitting as the dominant corrosion mechanism in high-Mn TWIP steels. An X-ray diffraction analysis of the surface revealed that the main corrosion products were hematite (Fe2O3), braunite (Mn2O3), and hausmannite (Mn3O4), and binary oxide spinels were also identified, such as galaxite (MnAl2O4) and jacobsite (MnFe2O4). This is due to the higher dissolution rate of Fe and Mn, which present a more active redox potential. In addition, a protective Al2O3 passive film was also revealed, showing enhanced corrosion protection. The highest corrosion susceptibility in both electrolytes was exhibited by the MBIP steel (30 wt.% Mn). Pitting corrosion was observed in both chloride and alkaline solutions.


Introduction
A single austenite phase steel that is stable at room temperature (RT) whose deformation mechanism, defined by the stacking fault energy (SFE), consists of the gliding of individual dislocations is known as twinning-induced plasticity (TWIP) steel [1][2][3][4][5]. However, the transformation of these twins can lead to local inhomogeneity, limiting the range of applications due to their increased susceptibility to hydrogen embrittlement [6,7]. Furthermore, the high content of Mn in these alloys severely impacts the corrosion performance due to the high dissolution rates observed for Mn [8]. Additionally, the straining process induces the formation of crystallographic microbands. Microbands consisting of geometrically necessary dislocations led to a high total dislocation density state during deformation, resulting in continuous strain hardening. This microband-induced plasticity (MBIP) is the origin of the enhanced mechanical properties of the steel [9,10].
Due to the needs of lightweight materials for the automotive industry in order to reduce both CO 2 emissions and improve fuel efficiency, special efforts has been made in alloy selection [5,6]. An austenitic TWIP steel alloy containing between 12-30 wt.% Mn was developed. The properties of this alloy perfectly match the requirements, as it is low density, has excellent mechanical properties, and has a good compromise between ductility

Materials and Methods
High-Mn TWIP steel specimens were obtained by the melting process of high-purity metals in an induction furnace under a protective argon gas environment. Ingots were forged at 1100 • C for 2 h and were homogenized at 1100 • C for 11 h. The ingots were then subjected to a thermal aging treatment at 600 • C for 18 h, followed by cooling in air at RT. The ingots were cut into slices that were 2.5 ± 0.2 mm thick using electro-discharge machining. Finally, the resulting slices were annealed at 1100 • C for 1 h in a tubular furnace with a constant flux of argon and cooled in air at RT. To determine the elemental composition, an S8 Tiger wavelength dispersive spectrometer was used. Table 1 shows the results from the X-ray fluorescence (XRF) for the three high-Mn austenitic steels studied and the SFE values obtained using stacking fault energy maps, as reported elsewhere [10]. In order to reveal the corrosion products of the TWIP steels after exposure, the samples were first epoxy mounted and then polished on a Struers Polisher Tegramin-30 following standard metallographic procedures. Specimens were ground up to 1200 grit using silicon carbide paper to remove native oxides and polished to a mirror finish using a colloidal silica suspension solution of 0.05 µm. Finally, samples were degreased in ethanol and air-dried.
Two different electrolyte test solutions were used-a neutral (pH 7) 3.5 wt.% NaCl solution and an alkaline (pH 14) 10 wt.% NaOH solution-to study the different corrosion behavior depending on the pH of the electrolyte [47]. Electrochemical measurements were performed using a flat electrochemical cell consisting of 3 electrodes: a working electrode which was the test specimen, the reference electrode which was a saturated calomel electrode (SCE), and a platinum auxiliary electrode. Triplicate measurements were obtained for all tests in a Gamry Reference 600 potentiostat. The corrosion potential (E corr ) value was obtained after steady state was reached at 25 • C. Afterwards, PP tests were recorded in a potential range between −200 mV < E corr < +1200 mV versus SCE at a scan rate of 0.1667 mV s −1 according to the ASTM G61-86 standard [48]. In addition, EIS tests were recorded after a 60 min relaxation time to stabilize the E corr , with an AC excitation signal of 10 mV rms . A frequency scan range between 10 5 and 10 −2 Hz was analyzed, acquiring 7 points per decade, following ASTM G106-89 standard [49].
Microstructural and corrosion product characterization was carried out by optical microscopy (OM) with an Olympus BX 51 TF. A crystallographic analysis was performed using X-ray diffraction (XRD) in a diffractometer equipped with a goniometer PW3050/60 (θ/θ) and an XPERT-PRO system. XRD patterns were obtained using a monochromatic radiation of Cu Kα with wavelength 1.54 Å, working at 40 kV and 40 mA, in a 2θ scan range from 20.01 • to 99.99 • , with a step size of 0.02 • /2θ, and at one step per 1 s. The XRD analysis of the TWIP and MBIP specimens was performed after the electrochemical corrosion tests to elucidate the composition of the oxide layer without removing the corrosion products. XRD peaks were assigned using the Powder Diffraction File (PDF) cards from the International Center for Diffraction Data (ICDD).

XRD Analysis
XRD patterns depict the presence of different corrosion products compounds formed on the three high-Mn steels. In Figure 1, the diffraction patterns obtained after exposure to 3.5 wt.% NaCl solution are shown, while Figure 2 corresponds to 10 wt.% NaOH solution.

Microstructure and Surface Characterization
The microstructure characterization by OM is presented in Figure 3a-c, which depict the austenitic structure of the three high-Mn steels. The OM cross-section micrographs for the three alloys TWIP1, TWIP2, and MBIP, exposed to the 3.5 wt.% NaCl and 10 wt.% NaOH electrolytes, are presented in Figure 4. For the samples exposed to the chloride environment shown in Figure 4, the most active alloy was the TWIP1 due to the severe pitting corrosion exhibited. This can be explained by the lower contents of Mo and Si that this alloy contains; Si imparts passivity by the formation of intermetallic materials, such as Fe 3 Al-Si, and increases the E pit , as well as extending the passive region [21,22]. In addition, molybdenum alloying modifies the polarity of passive film by generating molybdates and also creates a bipolar interface that promotes repassivation by the deactivation of pit growth. Molybdenum inhibits corrosion through forming MoO 3 oxide layers which convert to MoO 4 2− at the electrolyte/electrode interface, preventing the flux of OH − and Cl − ions into surface passive films and pits [25]. In contrast, the exposure to the highly alkaline electrolyte (10 wt.% NaOH) showed a more noble E corr compared to the samples exposed to chloride-containing solution (3.5 wt.% NaCl), in which TWIP2 is the most active alloy.

Microstructure and Surface Characterization
The microstructure characterization by OM is presented in Figure 3a-c, which depict the austenitic structure of the three high-Mn steels. The OM cross-section micrographs for the three alloys TWIP1, TWIP2, and MBIP, exposed to the 3.5 wt.% NaCl and 10 wt.% NaOH electrolytes, are presented in Figure 4. For the samples exposed to the chloride environment shown in Figure 4, the most active alloy was the TWIP1 due to the severe pitting corrosion exhibited. This can be explained by the lower contents of Mo and Si that this alloy contains; Si imparts passivity by the formation of intermetallic materials, such as Fe3Al-Si, and increases the Epit, as well as extending the passive region [21,22]. In addition, molybdenum alloying modifies the polarity of passive film by generating molybdates and also creates a bipolar interface that promotes repassivation by the deactivation of pit growth. Molybdenum inhibits corrosion through forming MoO3 oxide layers which convert to MoO4 2-at the electrolyte/electrode interface, preventing the flux of OHand Clions into surface passive films and pits [25]. In contrast, the exposure to the highly alkaline electrolyte (10 wt.% NaOH) showed a more noble Ecorr compared to the samples exposed to chloride-containing solution (3.5 wt.% NaCl), in which TWIP2 is the most active alloy.

Electrochemical Corrosion Analysis
PP scans were performed for the three alloys TWIP1, TWIP2, and MBIP in both electrolytes, 3.5 wt.% NaCl, and 10 wt.% NaOH. The cathodic kinetics were modified by the presence of alloying elements; it was observed that the oxygen reduction reaction (ORR) in 10 wt.% NaOH was promoted with the addition of Mo, as the exchange current density values were 4.32 × 10 −8 , 5.65 × 10 −10 , and 6.06 × 10 −7 A cm −2 for MBIP, TWIP1, and TWIP2, respectively. For the 3.5 wt.% NaCl solution, the exchange current density values were 3.82 × 10 −7 , 9.35 × 10 −10 , and 1.52 × 10 −8 A cm −2 for TWIP1, MBIP, and TWIP2, respectively. This exchange current density was obtained with the intersection of the cathodic Tafel slope and the ORR potential, leading to a current density value associated with the exchange current density. The anodic polarization curves depict an active-to-passive transition with an ill-defined Flade potential (Ef) peak (a shoulder-like shape), followed by a passive region. In the transpassive region, a breakdown pitting potential (Epit) corresponding to a sharp increase in the current density was obtained. The ORR was observed in neutral pH for potentials above 0.574 V vs. SCE according to the Nernst equation at RT (see Equation (1)):

Electrochemical Corrosion Analysis
PP scans were performed for the three alloys TWIP1, TWIP2, and MBIP in both electrolytes, 3.5 wt.% NaCl, and 10 wt.% NaOH. The cathodic kinetics were modified by the presence of alloying elements; it was observed that the oxygen reduction reaction (ORR) in 10 wt.% NaOH was promoted with the addition of Mo, as the exchange current density values were 4.32 × 10 −8 , 5.65 × 10 −10 , and 6.06 × 10 −7 A cm −2 for MBIP, TWIP1, and TWIP2, respectively. For the 3.5 wt.% NaCl solution, the exchange current density values were 3.82 × 10 −7 , 9.35 × 10 −10 , and 1.52 × 10 −8 A cm −2 for TWIP1, MBIP, and TWIP2, respectively. This exchange current density was obtained with the intersection of the cathodic Tafel slope and the ORR potential, leading to a current density value associated with the exchange current density. The anodic polarization curves depict an active-to-passive transition with an ill-defined Flade potential (E f ) peak (a shoulder-like shape), followed by a passive region. In the transpassive region, a breakdown pitting potential (E pit ) corresponding to a sharp increase in the current density was obtained. The ORR was observed in neutral pH for potentials above 0.574 V vs. SCE according to the Nernst equation at RT (see Equation (1)): where E O 2 /OH − is the reversible potential of the oxygen; E o O 2 /OH − is the standard reduction potential, being 0.401 V SHE for alkaline media; log OH − is a function of the pH; p 1/4 O 2 is the partial pressure of O 2 and equals 1 atm. This ORR is observed once the potential increases above the oxygen equilibrium line at 0.574 V vs. SCE for the neutral pH and 0.160 V SCE for the alkaline media. For increased potentials, the ORR rate also increases as more oxygen is reduced. This causes the nucleation of metastable pitting in the surface of the metal. The higher the anodic potentials above the oxygen equilibrium line, the higher the density of metastable pits, this can be seen in Figure 5a as wider and more frequent current shifts (metastable pitting, dissolution followed by repassivation). Surpassing the oxygen equilibrium line implies an enhanced dissolution rate, higher than the repassivation and the passive film growth, thus promoting the nucleation of stable pits. As more metastable pits grow, the chances for these pits to connect and form stable pits are increased, promoting the dissolution of the metal. The order of the anodic current passivity (i pass ) plateau was MBIP < TWIP2 < TWIP1, thus the passive layer of MBIP is the most stable, which may be attributed to the high passivating properties of the Mo alloying element [50] and of Al, which are higher that those of Cr and considerably higher than those of Mn and Fe [21,51,52]. Oscillations in the current density can be observed for the TWIP1 alloy in the beginning of the passive region and after the E f associated with metastable pitting (see Figure 5a). Hamada and Karjalainen reported that high-Al (8 wt.%) TWIP steel exhibited current density oscillations in the beginning of the passive region attributed to salt-film precipitation as a passivation mechanism, contrary to the spontaneous oxide film formation in a Cr-bearing steel [21]. The TWIP2 alloy improves the passivating properties with respect to the reference steel (TWIP1). A low Cr content enhances the passivity of the material. However, a high content (6-9 wt.%) has a detrimental effect on corrosion resistance [31]. This is because Cr causes phase-segregations, generating nucleation points for pitting corrosion [37]. Finally, the TWIP2 alloy also shows small current oscillations or the generation of metastable pits in the passive region (see Figure  5a). Using the Tafel extrapolation method, the corrosion current density (i corr ) and the Tafel slopes were determined, 2.63 × 10 −4 , 5.41 × 10 −5 , and 4.34 × 10 −4 A cm −2 for TWIP1, TWIP2, and MBIP, respectively, in 3.5 wt.% NaCl solution, as can be seen in Table 2. Using Faraday's law in Equation (2) (using 11.6 as the conversion factor), the corrosion rate was determined, yielding 0.00243, 0.00063, and 0.005 mm year −1 values for TWIP1, TWIP2, and MBIP, respectively: where CR is the corrosion rate, i corr is the corrosion current density, K is a constant that defines the units of CR (equal to 3272 to obtain mm/year), EW is the equivalent weight in grams/equivalent, ρ is density, and A is the exposed area in cm 2 . The increase in Al content yielded an increase in E corr and a decrease in i pass , whereas the increase in Mn alloying element did not produce a negative effect on the i pass , as can be seen in Figure 5b. This anomalous behavior, without a negative influence of an Mn content increase on the corrosion resistance, may be attributed to the amphoteric properties of the Al alloying element, which generates an unstable oxide layer in the alkaline (pH 14) 10 wt.% NaOH solution [36]. According to the Pourbaix diagram, Al generates a protective and stable Al 2 O 3 film in the 4-9 pH range [53]. As indicated above, the passive layer of Fe-Mn-Al-Cr steel is stable due to the spontaneous passivation the Al 2 O 3 film imparts, which is higher than Cr, Mn, and Fe [21,51]. In the case of the MBIP steel, the corrosion resistance may be enhanced by the 1.1 wt.% Mo alloying element (see Table 1), stabilizing the passive layer [50]. The increase in Al content yielded an increase in Ecorr and a decrease in ipass, whereas the increase in Mn alloying element did not produce a negative effect on the ipass, as can be seen in Figure 5b. This anomalous behavior, without a negative influence of an Mn content increase on the corrosion resistance, may be attributed to the amphoteric properties of the Al alloying element, which generates an unstable oxide layer in the alkaline (pH 14) 10 wt.% NaOH solution [36]. According to the Pourbaix diagram, Al generates a protective and stable Al2O3 film in the 4-9 pH range [53]. As indicated above, the passive layer of Fe−Mn−Al−Cr steel is stable due to the spontaneous passivation the Al2O3 film  Table 2. Electrochemical parameters obtained from the potentiodynamic polarization curves in Figure 5, for TWIP1, TWIP2, and MBIP steels in 3.5 wt.% NaCl and 10 wt.% NaOH solutions. Using the Tafel extrapolation method, the corrosion current density (i corr ) and the Tafel slopes were determined. The i corr was 1.48 × 10 −4 , 2.65 × 10 −5 , and 1.27 × 10 −4 A cm −2 for TWIP1, TWIP2, and MBIP, respectively, in 10 wt.% NaOH. The Tafel slopes presented in Table 2 showed higher cathodic kinetics, indicating the overall electrochemical reaction was controlled by the oxygen reduction reaction at the cathode, and the steadystate limiting current density was achieved around 10 −2 A cm −2 , corresponding to the maximum diffusion current density in the oxygen reduction reaction (ORR). The corrosion rates were 0.00172, 0.00031, and 0.0015 mm year −1 for the TWIP1, TWIP2, and MBIP, respectively; this is in accordance with the results observed in the OM, showing lower corrosion rates for the samples exposed to 10 wt.% NaOH. The electrochemical transfer coefficients can be obtained and discussed using Equations (3) and (4) [54]: where α a and α c are the anodic and cathodic transfer coefficients, respectively; R is the ideal gas constant (8.314 J mol −1 K −1 ); T is the temperature in K; n is the number of electrons; F is the Faraday constant (96,485 C mol −1 ); and β a and β c are the anodic and cathodic Tafel slopes in V/dec, respectively. Table 2 summarizes the electrochemical parameters obtained by PP, showing the highest charge transfer coefficient for MBIP in 10 wt.% NaOH, while TWIP1 presents the highest in 3.5 wt.% NaCl. In the case of the TWIP2 steel, the α a and α c values are in the same range independently of the electrolyte, thus indicating a passive-like behavior. The low value of 0.00031 mm year −1 for the TWIP2 steel may be attributed to the low presence of Al (5.2 wt.%) and the high Cr content (5.1 wt.%). As indicated previously, this higher Cr content enhances the corrosion resistance [37]. Moreover, the presence of Si (2.8 wt.%) has a beneficial influence on the corrosion resistance, which favors the formation of a stable passive film and increases the E pit . Finally, the passivation mechanism of the three high-Mn steels tested in the 10 wt.% NaOH solution may be due to the spontaneous oxide layer formation in Al-bearing steels. Figure 6 represents the Nyquist plots for the three tested high-Mn steel alloys, where Figure 6a shows the corrosion behavior in 3.5 wt.% NaCl solution and Figure 6b in 10 wt.% NaOH solution. Two semicircles are observed, which correspond to the passive film and double-layer interfaces. The Bode plots are presented in Figure 7, a two-time constants electrochemical process is shown, identified by the phase angle inflexion. The EIS results were modeled by the electrical equivalent circuit (EEC) of Figure 8 to describe the electrochemical properties of the interfaces of high-Mn TWIP steels. The EIS results obtained in both corrosion media, chloride and alkaline, were modeled with the same EEC. The EEC depicted in Figure 8 is composed of two time-constants (R//CPE) representing a hierarchically distributed circuit, where the first time-constant, found at high frequencies, corresponds to the passive film-electrolyte interface (R film //CPE film ), where a non-uniform current distribution along the interface is denoted by the constant phase element of the passive film (CPE film ) and the resistance of the passive film (R film ), and the second time constant, found at low frequencies corresponds to the electrochemical double layer represented by (CPE dl ), including the charge transfer resistance (R ct ), which is inversely proportional to the corrosion rate (v corr ), and denotes an electrode process (R ct //CPE dl ) [55][56][57]. The ECC also accounts for the solution ohmic drop denoted by the electrolyte resistance (R s ). The CPE accounts for the non-ideal capacitance response of an active electrode, and its impedance is described by Z CPE = (Y) −1 (jω) −n , where Y is the admittance (S cm −2 s n ), ω is the angular frequency (rad s −1 ), j is the imaginary number, and n is a dimensionless variable that represents the non-ideality of the CPE. The values of n range from 1, which would make the CPE an ideal capacitor, to 0 which will represent an ideal resistor and, where values of 0.5 could show a diffusion process represented by a Warburg element [38,[56][57][58][59][60].
The Nyquist plots show a good fitting, as the experimental data, denoted by empty symbols, and the calculated data using EEC and denoted by crosses present a consistent matching for all three alloys in both solutions. Table 3 summarizes all the values from the EEC elements, where the error of each parameter was kept under 10% and the goodness of fit (χ 2 ) was in 10 −3 for all the fitting curves. In addition, the robustness of the experimental impedance data was evaluated using the Kramers-Kronig (KK) transforms [58,61]. Figure 9 shows an example of the comparison between the experimental EIS data from Figure 6 for the TWIP1 steel in the 3.5 wt.% NaCl solution and in the 10 wt.% NaOH solution and those obtained by means of the KK transforms. The correlation between the experimental and the KK-transformed data is excellent as can be seen in Figure 9, confirming the robustness of the EIS data and, therefore, its validity to model the high-Mn TWIP steel electrochemical corrosion process.
R s values of 26.0-28.1 and 30.1-32.1 Ω cm 2 are obtained for all three high-Mn steels in both electrolytes, 3.5 wt.% NaCl, and 10 wt.% NaOH solution, respectively. Thus, this shows that the electrolyte conductivity is similar. The R film stays in the same order of magnitude for both solutions, slightly changing between alloys ranging from 142.5 to 607.7 Ω cm 2 for the NaCl solution and from 136.6 to 295.1 Ω cm 2 for the NaOH solution. The pseudo-capacitance of the surface oxide film (Y film ) is in the µS cm −2 s n1 , which is in the typical order of magnitude for passive films, for both solutions, being higher in the NaOH than in the NaCl by almost double the value, indicating a thinner film in the case of the NaOH. Accordingly, n 1 remains withing the same range from 0.492 to 0.588 for the NaCl and from 0.466 to 0.607 for the NaOH. The R ct in NaCl solution significantly changes between samples, having the highest impedance value, thus more protective, for TWIP2 with 21593 Ω cm 2 , followed by TWIP1 and MBIP with 2220 and 952 Ω cm 2 , respectively. There is a reduction of one order of magnitude among TWIP2 and TWIP1, and a further order of magnitude reduction among TWIP1 and MBIP. This same trade is seen in the NaOH solution where TWIP2, TWIP1 and MBIP have 11310, 3324 and 555 Ω cm 2 respectively. Finally, the Y dl and n 2 , remain barely unchanged from sample to sample and solution, being in the 0.01 µS cm −2 s n2 order of magnitude and 0.711 to 0.847 range, respectively.        Table 3. EIS fitting parameters for high-Mn steels in 3.5 wt.% NaCl and 10 wt.% NaOH electrolyte solutions at 25 • C (see Figure 6), using the electrical equivalent circuit (EEC) model of Figure 8.  Table 3. EIS fitting parameters for high-Mn steels in 3.5 wt.% NaCl and 10 wt.% NaOH electrolyte solutions at 25 °C (see Figure 6), using the electrical equivalent circuit (EEC) model of Figure 8.   The i corr was estimated through the Stern-Geary relationship, i corr = B/R ct , where B is a constant defined by B = (β a β c )/2.3(β a + β c ), β a, and β c are the anodic and cathodic Tafel slopes, respectively, in the PP tests (Figure 5a,b), B values can be seen in Table 2. Finally, R ct has been defined above; see Table 2. The corrosion rate determined using Faraday's law was 0.27, 0.01, and 0.67 mm year −1 for TWIP1, TWIP2, and MBIP in 3.5 wt.% NaCl solution, respectively, and 0.23, 0.03, and 0.29 mm year −1 for TWIP1, TWIP2, and MBIP in 10 wt.% NaOH solution, respectively. These findings are higher than the corrosion rate results yielded by the PP experiments of Figure 5. Furthermore, the worst performing alloy was found to be MBIP, which is in accordance with PP curves. This might be due to the effect of Mn, promoting a higher dissolution rate.

Rs
As previously described, CPE is a non-ideal element which represents a branched ladder R//C network, and hence it is not possible to directly measure the capacitance. In order to get the effective capacitance (C eff ), the resistance has to be also taken into account for correcting the value. The equation proposed by Brug et al. enables the calculation of the accurate value of the C eff of the double layer (C eff,dl ), which uses the resistance of the R ct and the R s (see Equation (5)) [59].
The obtained values for the C eff,dl and R ct parameters for the three high-Mn steels studied in the 3.5 wt.% NaCl and 10 wt.% NaOH solutions are depicted in Figure 10. It is observed that the higher the R ct the lower the C eff,dl , which is in good agreement, as the higher the impedance and the lower the capacitance the more protection the film imparts [57]. The TWIP2 steel shows the lowest corrosion kinetics as it shows the highest R ct and the lowest C eff,dl followed by TWIP1 and MBIP, this behavior is seen in both solutions 3.5 wt.% NaCl and 10 wt.% NaOH. From the trend of decreasing the impedance and increasing the capacitance with addition of Mn in the TWIP alloy, 22.6, 28 and 30 wt.% respectively, for chloride and alkaline solutions, it can be concluded that increasing the Mn content leads to lower corrosion properties. The results from the AC and DC techniques are in good agreement and prove that the TWIP2 alloys exhibit more noble corrosion behavior.

Conclusions
• The three high-Mn steels tested showed austenitic microstructures. After electrochemical experiments, the optical micrographs showed pitting and uniform corro-

Conclusions
• The three high-Mn steels tested showed austenitic microstructures. After electrochemical experiments, the optical micrographs showed pitting and uniform corrosion for all samples in both chloride and alkaline solutions.

•
The X-ray diffraction results indicated that the main surface corrosion products identified were Fe oxide (Fe 2 O 3 or Fe 3 O 4 ), Mn oxide (MnO 2 , Mn 2 O 3 , or Mn 3 O 4 ), MnAl 2 O 4 , and MnFe 2 O 4 . This is due to the higher dissolution rate of Fe and Mn, which present a more active redox potential. In addition, a passivating Al 2 O 3 oxide film was revealed.

•
The PP scans showed that the cathodic kinetics decreased as the content of Mn increased. This behavior was interpreted in terms of the catalytic properties of the alloys towards the oxygen reduction reaction (ORR). The anodic branches depicted an active-to-passive transition defining a shoulder-like followed by a passivation region, an E pit , and the evolution of oxygen. In the 10 wt.% NaOH solution, the anodic branch was stable without current density oscillations, which was attributed to the spontaneous passivation imparted by the Al 2 O 3 film. Contrarily, in the 3.5 wt.% NaCl solution current density oscillations were observed mainly in TWIP1 and TWIP2 and were attributed to a salt-film precipitation passivation mechanism. The corrosion rate was found to be higher in both electrolytes for MBIP because of the higher Mn content, while the lowest corrosion rate was recorded for the TWIP2 due to the presence of Mo and the higher Cr content imparting passivity.

•
The EIS results revealed a capacitive behavior with two-time constants, one at high frequencies for the passive layer and one at low frequencies for the corrosion process. The results are in agreement with the PP scans showing the lowest corrosion rate in TWIP2 and the highest in MBIP. Informed Consent Statement: Not applicable.

Data Availability Statement:
The raw/processed data required to reproduce these findings cannot be shared at this time as the data also forms part of an ongoing study.